285 45 15MB
English Pages 305
236 119 4MB Read more
429 120 6MB Read more
257 91 3MB Read more
J.F. Koksma's paper that extends the Erdos-Turan inequality to the multidimensional setting.
341 100 22MB Read more
S O M E
f I 0 IT
S ! ? B I I S
0 s » n o s
t o o l
A Thesis e u b m i t t M to the Dniversity of Glasgow for the Degree of Doctor of Philosophy in The faculty of Science
Colour* Chemistry Research Laboratory, Technical Chemistry Department, Royal Technical College, Clasgow. Bated the
fasant Be Chipalkatti
ProQuest Number: 13838114
All rights reserved INFORMATION TO ALL USERS The quality of this reproduction is d e p e n d e n t upon the quality of the copy subm itted. In the unlikely e v e n t that the a u thor did not send a c o m p le te m anuscript and there are missing pages, these will be noted. Also, if m aterial had to be rem oved, a n o te will ind ica te the deletion.
uest ProQuest 13838114 Published by ProQuest LLC(2019). C opyright of the Dissertation is held by the Author. All rights reserved. This work is protected against unauthorized copying under Title 17, United States C o d e M icroform Edition © ProQuest LLC. ProQuest LLC. 789 East Eisenhower Parkway P.O. Box 1346 Ann Arbor, Ml 4 8 1 0 6 - 1346
P-P. Acknowledgments. Preface. Abstract of Thesis. Is
1 - 19.
.... ; .............
Results and Discussion......................... 20 (A)
Sorption from aqueous solution....... 20 - 57 (i) ( ii)
( iv )
Isotherms for phenol on drawn and undrawn n y l o n .........
Isotherms for resorcinol, aniline, benzoic acid, and benzene sulphonic acid on nylon ........................
Studies of rates of sorption of phenol and benzoic acid from aqueous solution on n y l o n ..........................
C ONCUJSIQHS. . .
II s Eesults and Discussion (continued) (B)
Sorption from vapour phase (i) (ii)
Sorption from vapour phase (continued) (i) (ii) (iii) (iv) (v) (vi) (vii)
Water, methyl alcohol and ethyl alcohol on drawn n y l o n .......
Phenol vapour on nylon and wool ...............................
Acetic acid vapour on nylon and wool ..........................
-naphthol and alizarine vapours on nylon and wool ..........
Benzoic acid vapour on nylon and wool .....................
Aniline vapour on drawn nylon
Acetic acid vapour on wool, variously treated ................
II : Results and Discussions (continued) (D)
Isotherms from vapour phase
......... . . 1 2 3 - 1 40(a)
(i) Water, methyl alcohol and ethyl alcohol on drawn n y l o n ........
(ii) Water isotherms on wool, variously t r e a t e d ....................
(iii) Conclusions ......................... Appendix
:The energetics of a d s o r p t i o n ........
:Adsorption k i n e t i c s .................. 162
:The adsorption e q u i l i b r i u m ........
:Theories of adsorption and the textile f i b r e s ....... ...... . 182
2 (Materials and
Misceue n b ous) TflisuLflTGD
•* ......... ..........
Ackhowle dgmen t s
Thanks are due to many members of the staff in The Technical Chemistry Department of the Royal Technical College, including the glasshlower, Mr. Barbour, and Messrs.
Clunie and Scally of
the workshop, for their assistance in constructing the apparatus used in the present research. The work was carried out under the guidance of Dr. C.H. Giles and Prof. W. M. Gumming, O.B.B., F.R.S.E., and the author is grateful to them for all their help.
The author feels particu-
slarly grateful to Dr. C.H. Giles, who had a
influence. The author also wishes to thank Prof. P. D. Ritchie, successor to Prof. Gumming, for his kind help and suggestions. Part of the work on the sorption of aqueous phenol on nylon was done by Miss Margaret Laidlaw and Miss Patricia Brand, and the author is indebted to them for their assistance. Pinally, the author wishes to thank the management of the Delhi Cloth and General Mills Co.Ltd., D elHi, India, for granting him the necessary leave of absence, and funds to carry out the present work.
V. 8. C .
This research was originally undertaken with a view to studying sorption on textiles from the vapour phase.
required the use of high vacuum technique and as some free time was available in the initial stages of building up the apparatus, sorption from aqueous solution was also studied. There are two features of the experimental technique which need particular mention.
Firstly, the use of Pyrex glass
spirals for sorption measurements from the vapour phase.*
smunication to "nature” in this connection awaits publication. Secondly, the technique of studying vapour phase sorption at j
temperatures as high as 120°G to 150°C on textile fibres is some-; swhat novel.
It was found that nylon and wool are not damaged
even at such high temperatures, if under a high vacuum. It is hoped to publish the present work in one or more papers in one of the scientific journals.
P v U A c /•*««, 6, l *4'ov
ABSTRACT Off THESIS
A review is made of the present knowledge of the subject of sorption in relation to textile fibres and it is pointed out that the exact role of the amino and amido groups of the polyamide or protein fibres in their behaviour with hydroxylic compounds, acids or acid dyes is not yet fully understood.
The experiments were
planned and the results are discussed to throw additional light on this behaviour. Sorption has been studied both from aqueous solution and from the vapour phase.
The sorbates used were hydroxylic, phenolic or
The fibres used as sorbents included drawn,
undrawn and powdered nylon, and untreated, acid treated, dyed and , i
deaminated wool, respectively. Sorption from aqueous solution The methods used for the study of sorption from aqueous solu t i o n are those commonly employed, with the difference that in this work, the material
sorbate ratio (and not the material
liquor ratio) was maintained constant.
Such a procedure is more
in keeping with the requirements of the law of mass action.
equilibrium concentration of the sorbate bath is expressed as ’relative concentration* which is defined as the actual concen t r a t i o n divided by the solubility at the temperature under study. It is shown how results so expressed are thus made easier of
II Abstract of Thesis
interpretation and more consistent.
The following conclusions
Resorcinol has a greater affinity towards nylon than
In spite of its extremely low solubility in water,
benzoic acid shows an appreciable sorption on nylon, whereas benszene sulphonic acid shows none.
It is concluded that the formei
combines with nylon by hydrogen bonds at the -JSIH.CO- groups. (iii)
A formula is derived for the isotherm of phenol on the
assumption that the molecules of phenol behave as gas molecules and the solvent water is in effect an indifferent medium.
derivation of the formula then follows the kinetic considerations of Langmuir and the isotherm equation is similar to his equation* Prom a study of the isotherms at different temperatures, heats of reaction of phenol on drawn and undrawn nylon are calculated and it is shown how swelling and contraction complicate the inter pretation. (iv)
T^e data of rates of sorption have been utilised to cal
sculate the activation energy of a sorbate on the fibre under insvestigation.
This is done by drawing slopes to the rate curves
at the zero point and thus calculating the velocity constants at different temperatures.
The effect of variations in solubility
Ill Abstract of The ►sis
with temperature are taken into account by dividing the velocityconstant by the solubility at the given temperature.
of activation thus calculated are given for phenol and benzoic acid.
The activation energy of phenol on drawn nylon is about
18.000 cal/g.mol. whereas that on undrawn nylon is about 24.000 cal/g.mol.
The energy of activation of benzoic acid on
drawn nylon is about 25,000 cal/g.mol. (v)
Isotherms of aqueous aniline on drawn nylon revealed a
appreciable sorption of this compound by the fibre.
It was later
discovered that aniline from the vapour phase is not adsorbed by the fibre.
It is suggested that aniline combines with nylon not
directly but through a bridge of water molecules. Sorption from vapour phase McBain and Bakr* s spring balance has been used for the study of sorption from the vapour phase.
The cleaning of the fibre
surface was done under high vacuum (1(T^ mm.). glass have given very satisfactory service.
Spirals of Pyrex The following
conclusions are drawn:(i)
Water and methyl alcohol are attached to nylon and wool
by hydrogen bonding on the -SHOO- groups.
The present results
thus seem to be more in agreement with Oassie*s views rather than
IV Abstract of Thesis
with those of Frey and Walter, who assume that the water combines with the polar side chains. (ii)
Water isotherms on untreated wool, acid treated wool,
dyed wool and deaminated wool, respectively,
show the remarkable
result that all these fibres give identical isotherms.
c r e a s e in the surface area or the number of amino groups has therefore no direct bearing on the course of water sorption. (iii)
Hates of sorption of dry acetic acid vapour on the di
sferent samples of wool mentioned above reveal that the dyed sample (Solway Blue B.S.) shows a far lower rate and the sphuric acid-treated one a far higher rate, than one.
The points of attachment
of the dye molecules and the
acetic acid molecules appear to be identical. (iv)
Further, sorption and desorption rate studies with
acetic acid and benzoic acid vapours on wool and nylon show that the amino group does not exert any specific influence on the course of the reaction, and hence it is concluded that the comsbination is probably by hydrogen bonds and not by salt formation* (v)
In the case of phenol, /3-naphthol, benzoic acid and
alizarine, rates of sorption and desorption were studied at tempJeratures varying from 60°G to 150°C.
An important point is
that successive sorptions and desorptions cause a loosening of the fibre structure and the fibre thus shows an increasing
V Abstract of Thesis capacity to sorb.
This is true of both wool and nylon.
sorption in all these cases is quite high and it must be concluded that these substances have a great affinity for the two fibres. The mode of combination is presumably by hydrogen bonds.
energies of activation for the combination with nylon and wool range from
Adsorption is considered theoretically both from the kinetic and the thermodynamic angle.
Various theories of
adsorption are discussed and consideration of the various general theories is made with special reference to textile fibres.
is suggested that the "non-rigidity" of the fibre surface is bound to make impossible a perfect fit of experimental results to any theory.
I I 1
1 I 0 P U C T I 0 I ,, J
Sorption studies are of immense value to the understanding of general theoretical chemistry, e.g. in j^eterogeneons catalysis colloid science, the stru.ctu.re of active surfaces, the separation and purification of gases, etc.
For the textile chemist, the
subject is important because it is an aid to the understanding of the internal structure of fibres as well as their behaviour towards dyeing and finishing chemicals.
The scope of, as well
as the need for, more research in the subject is therefore easily appreciated. The earlier workers - in the late 19th or early 20th centur:ies - were greatly hampered by the lack of sufficient data to understand the structure of fibres or their behaviour towards dyes and chemicals.
Their work now appears vague and empirical.
But fortunately for us great advance has been made in the knowledge of theoretical textile chemistry during the last 25 to 30 years.
This advance has closely followed those made in other
branches of chemistry.
Thus the conception of electronic
valency, the x-ray study of crystalline bodies, new knowledge of the constitution of cellulose and proteins, modern theories of electrolytes, the methods of molecular analysis by means of infra* red spectrum, etc., have all aided the m o d e m textile chemist to j design more precise experiments in his own field.
A review of relevant literature The literature published by investigators interested in fibrefchemistry, shows three main trends in their work:(i)
Elucidation of the physical and physico-chemical st
:ture of the fibres and correlation of their physical and mechan :ical properties with their chemical behaviour. (ii)
Formulation of a general theory of the mechanism of
dyeing and other textile finishing processes. (iii)
Use of the theoretical basis provided by modern ideas
in the fields of Jhemical kinetics and chemical Thermodyanamics. On the structural side Haworth (l) laid a foundation for cellulose chemistry by developing the cyclic formula for glucose Similarly Fischer*s work on proteins, peptides and amino acids greatly advanced our understanding of the proteinous fibres. Following Bragg's technique of building up molecular models with the help of x-ray data, Sponsler and Dore (2) established the alternate 1:1 and 1:4 linkages in glucobiose.
Mark (3) and Polanyi (4) established the question of laterel spacings and put the "molecular chain" theory of cellulose on a firm basis.
The fact that these molecular chains co'uld form
bundles by lateral cohesion was established by Mark and Meyer (Loc.cit) and by Hengstenberg and Mark (5).
This view received
further support from the work of Boulton, Dellph, Fothergill and
I IrT E 0 D U 0 T I 0 H Morton (6) who pictured cellulose as a threedimensional network of more or less parallel chain molecules producing "crystalline1* regions when orderly arranged and "amorphous" regions when arranged in a disorderly fashion. Similar fundamental work was taken up by many investigators for studying the internal structure and molecular arrangements within the wool fibre.
Of particular interest is the work of
Astbury who explained the elastic properties of the wool on the basis of its x-ray structure (7) and established that stretching causes an axial orientation and produces pronounced regularity* Similar evidence for crystalline and amorphous regions in Nylon has now been published by Burns & G-arner (8).
Marsden (9) and
Meridith (10) in two lectures have recently made a very signifiscant contribution by simply and lucidly exposing the importance of the "crystalline and amorphous" nature of fibres and their influence on their dyeing and chemical properties. As a result of all this work we can now form a general picsture of the internal arrangement of molecules within a textile fibre.
This picture may be briefly summarised as follows
(i), Textile fibres consist of molecules which are very long and thin. (ii)
These molecules are held together by lateral cohesive
I N T R 0 D II C T I C ]f
When the lateral arrangement is of a regular order,
the portion of the fihre shows crystalline nature;
mechanical extension and also chemical action. (iv)
When the lateral arrangement is irregular the portion
of the fihre shows amorphous characteristics.
It is easily
attacked hy chemicals and acquires ruhher-like properties - i.e. it offers less resistance to extension. (v)
The crystalline and amorphous regions do not necessar
i l y hear a fixed relation with each other.
Depending on the
previous history, the fihre may show more or less crystallinity. (vi} nature.
The lateral cohesive forces are of a weak or secondary The modern conception of the hydrogen hond (11) has
heen widely applied and used hy the textile chemists $n this connection. All the x-ray evidence of fihre structure is no douht con vincing.
But the real difficulty is to try and provide chemi-
:cal evidence to support the x-ray structure. we may mention one case.
As an example,
Speakman (12) , Ender and Mtiller (13) ,
Harris (14), and various other workers took it as established that the capacity of wool for combining with acids and acid dyes has a stoichiometric relationship with the amount of its free amino groups.
But Asthury and Dawson (15) showed conclusively
I N T R O D U C T I O N that the amino groups in the crystalline regions of wool do not show any signs of combination with dyes.
Speakman (16) suggests
that the electric charges on the amino groups in the crystalline regions are strong enough to attract and hold together dye mole:cules at a distance and that the dye particles need not actually go near the amino groups in the fihre at all.
does not appear, to be very convincing. Speakman’s contribution to the understanding of Wool Chemisstry has however been extensive (17, 18i 19, 20, 21); are:-
his work on the acid base combining capacity of wool, the
sulphide linkage in wool, the relation between its swelling pro sper ties and its physico-chemical structure.
Probably one of
the most important among his recent contributions is his paper in the Journal of The Society of Dyers & Colorists (22).
paper he and his colleague (Peters) have applied the Donnan equi librium principle to the data of his own titration curves and those of Milton, Harris and his colleagues (23).
Peters, after pointing out the defects of Harris’ theory as well as the improved theory of Gilbert and Rideal (24) have clearly shown how the new application of Donnan’s principle explains all the published facts.
In Harris’ experimental data, the titration
curves for hydrochloric acid on wool gradually shifted their position with respect to the pH axis with varying amounts of
I N T R O D U C T I O N pptassium chloride added to the hath.
But the two authors have
shown that the internal pH within the wool fihre is not the same as the external pH and when this is calculated and the pH • absorption curves are redrawn, all the curves coincide with each other.
As far as the theory of the combination of strong acids
with wool is concerned, this is indeed a great step forward. The part played by the amino group in dyeing has been inves tigated by Skinner and Yickerstaff (25) from a new angle.
have determined the sorption isotherms of three dyes from aqueous solutions for wool and have indicated that perhaps the dyeing mechanism in protein fibres is more complicated than mere salt formation.
Carlene, Fern and Vickerstaff (26) studied the com
bination of acid dyes with amino and amide groups in nylon fibre and found the behaviour of these groups similar to those in wool. Some interesting data on the dyeing of direct dyes on nylon have been published by Boulton (27).
His observation that nylon
can be dyed by direct dyes from a neutral bath as well as by direct or acid dyes from an acid bath is interesting.
that nylon can show a dual dyeing behaviour, i.e. dye combines as in cellulose on the one hand and as in wool on the other.
important observation made by him is that nylon yarn dyed with direct dyes exhibits dichroism when examined in polarised light,
As in cellulose, residual valency forces therefore seem to take some part in nylon dyeing.
The heat changes accompanying dye-absorption or acid absorp t i o n by protein fibres have been calculated by various workers. Thus Harris (28) has studied the effect of temperature on the ti tration curve for hydrochloric acid on wool and from the heat calculations finds support to the idea that -NH^ and -COOH groups in wool are completely ionised;but his data could not be taken as giving proof either for or against Speakman’s salt-linkage theory. Speakman and Scott on the other hand (29) determined the heats of reaction for hydrochloric acid and acetic acid on wool calorimetsrically, and from the low heat values obtained, they concluded that the work required to break the salt linkages in wool has to be spent by the incoming combining ions and so the value of heat of reaction is low.
This they considered an indirect proof of
the salt linkage theory. It is to be noted here that from the point of view of the work presented in this thesis, this controversy on the exact role of the amino and amido groups of wool and nylon in their combina ction with acids or acid dyes is of particular interest.
discussing the experimental data, an attempt will be made to throw some light on this point. Mention must be made of one more piece of work by Marsden & Urquhart published in 1942. (30).
These authors studied the
absorption of phenol by cellulose acetate and clearly demonstrated
I II T E 0 D U C T I 0 I how the absorption of phenol was closely connected with the absorption of water itself.
The swelling action of phenol is
explained or assumed to be due to hydrogen bonding between the phenolic oxygen and the carbonyl group of the cellulose acetate. The conception that hydrogen bonding might also play an important role in sorption of dyes and chemicals by textiles, has gained considerable support since then. From what has been said in the foregoing, it will be clear that data of sorptions from solution have a very important role to play.
But these data are not sufficient.
There are some inher-
ient difficulties which make it necessary to resort to many assumptions.
Moreover when sorption is studied from solutions,
the varying solubilities of the solutes at different temperatures makes the effect of temperature on the rate and equilibrium of * sorption reaction difficult to ascertain.’1' The heat calculation from such data cannot be taken without some reserve.
the part played by the solvent molecules themselves in changing the structure of the fibre or in influencing the course of sorption has always to be ignored for mathematical simplification - and this may not be always right. As a result of this, the study of vapour sorption on textiles has attracted the attention of many textile investigators in recent times. ..£>& jGffciW _ liwP&kl#if£ £*} W
N ‘ f L 4} W